Absorption and scattering properties of carbon nanohorn-based nanofluids for direct sunlight absorbers
© Mercatelli et al; licensee Springer. 2011
Received: 4 November 2010
Accepted: 4 April 2011
Published: 4 April 2011
In the present work, we investigated the scattering and spectrally resolved absorption properties of nanofluids consisting in aqueous and glycol suspensions of single-wall carbon nanohorns. The characteristics of these nanofluids were evaluated in view of their use as sunlight absorber fluids in a solar device. The observed nanoparticle-induced differences in optical properties appeared promising, leading to a considerably higher sunlight absorption with respect to the pure base fluids. Scattered light was found to be not more than about 5% with respect to the total attenuation of light. Both these effects, together with the possible chemical functionalization of carbon nanohorns, make this new kind of nanofluids very interesting for increasing the overall efficiency of the sunlight exploiting device.
78.40.Ri, 78.35.+c, 78.67.Bf, 88.40.fh, 88.40.fr, 81.05.U.
Heat exchange devices suffer a serious limitation due to the relatively low thermal conductivity of conventional fluids. Because of solid materials have typical thermal conductivities order-of-magnitude higher than that of liquids, the possibility to add some amount of solid particles to conventional heat transfer fluids has been widely investigated in the literature [1–4] since the pioneering works done in seventies [5, 6]. Anyway, as the thermal conductivity enhancement is dependent on the surface area-to-volume ratio, the use of nanometer-sized, non-spherically shaped particles offers the largest advantage.
In the fields of the research and technology involving the exploitation of renewable energies, solar thermal collectors have gained an increasing role in the last years . The so-called "thermal" sunlight exploiting devices are heat exchangers that transform the energy of solar radiation to internal energy of some exchange medium. Typically, solar energy is absorbed by black-surface tubes (typically, a black-painted or oxidized surface in tight thermal contact with the tubes) , but this configuration entails various limitations. Therefore, alternative concepts have been addressed like the use of black particles suspended in gases  or in liquids as both solar radiation absorbers and heat transfer medium. In fact, carbon particles in gases have been demonstrated to be very efficient for devices operating in the high temperature range , whereas collectors employing black liquids within a transparent tube result advantageous in the low and medium temperature working range . Conventional black liquids are based on organic inks or Indian ink, but they show serious drawbacks because of the light-induced degradation and thermal degradation at the operating temperatures, instability of solutions during time and fouling of inks on the internal side of exposed surfaces.
For these reasons, the use of nanofluids in solar thermal collectors is being investigated. Different spherically shaped materials, such as aluminium  and copper  have been added to different base fluids and characterized in terms of their performances for improving heat transfer efficiency. Materials with higher surface area-to-volume ratio due to a markedly aspherical shape have been investigated as well, like multiwall [12–15] and single-wall  carbon nanotubes (CNTs). CNTs are characterized by themselves by a very high thermal conductivity [12, 17, 18] and, also when suspended in fluids, they have been demonstrated to be very promising to enhance the heat transfer within the fluid [14–16, 19]. Carbon nanohorns (CNHs) are the latest to be discovered in the family of carbon-based nanostructured materials . They have a large surface area and a large number of cavities , and therefore appear promising for a variety of applications, such as electrode material in fuel cells , gas storage material , and carrier vehicles for delivering therapeutic drugs, genes or proteins [24–26].
A single-wall carbon nanohorn (SWCNH) consists of a single layer of a graphene sheet wrapped into an irregular tubule with a variable diameter of generally 2-5 nm and a length of 30-50 nm; the tips of the nanohorns are cone-shaped with an average angle of about 20° [27–29], corresponding to five pentagonal carbon rings at the tip of the tubule. The SWNHs assemble to form roughly spherical aggregates of mainly three types, known as dahlias, buds and seeds , depending on the synthesis conditions [20, 30]. Among these possible aggregation states, the dahlia-flowerlike morphology has emerged as an interesting material within the family of carbon nanostructures  because it can be produced in high quantities and with high purity [20, 30, 32]. In fact, the critical points that differentiate CNH from CNT are their high purity due to the absence of metal nanoparticles (typically Fe and Co) used to catalyze nanotube growth during their production, the heterogeneous surface structure due to their highly strained conical ends, and finally the aggregation in spherical superstructures, typically ranging between 50 and 100 nm. Moreover, the rough surface structure of CNH aggregates with minimum Van der Waals interactions between the superstructures gives rise to better dispersion of CNH in liquid media  and a much longer time stability of their suspensions. Moreover, a very important property in view of their potential use with respect to CNTs arises from the metal-free structure of nanohorns that makes their cytotoxicity negligible, as has been widely confirmed by experiments on mice and rats . This makes the use of SWCNH very appealing in all applications where the handling by operators is needed or when accidental leakages into the environment are possible.
Up to now, among the physical properties of nanofluids, the ones which usually are evaluated in view of practical applications are thermal conductivity [1–6, 11] and pool boiling heat transfer [35–37]. However, as nanofluids appear promising for thermal solar energy applications, it is also important to carry out investigation of their optical properties allowing to assess their potentialities as direct sunlight absorbers.
Very recently, aqueous suspensions of SWCNH have been studied in view of this possible use . However, in solar thermal collectors, water is often replaced by glycols or water/glycol mixtures, to protect against freeze damage and/or to increase the temperature for high temperature solar collectors, since glycols have lower freezing point and higher boiling point with respect to water.
Therefore, in this article we comparatively evaluated the thermal stability and the spectral absorption properties of water-based and glycol-based SWCNH suspensions, in the perspective to use them as direct absorber fluid in a sunlight collecting device. In addition, to evaluate the relative weight of scattering processes over the overall light extinction phenomenon, the absorption and scattering coefficients of SWCNH aqueous suspensions were separately measured with the utilization of a simple and precise technique. This allowed to assess the reliability of the measured transmittance data. This extensive analysis of SWCNH nanofluids can optimize their use, providing useful information for the system dimensioning.
Results and discussion
Sample preparation and structural characterization
A patented method (Carbonium Srl)  was used to produce very pure SWCNHs. This method demonstrated excellent capability and, differently from other methods commonly used, could be easily scaled up for massive production .
SWCNHs were mechanically dispersed in water and ethylene glycol by a high pressure homogenizer. In the case of water dispersions, the use of a dispersant resulted necessary and the sodium n-dodecyl sulphate (SDS, 99%, Alfa Aesar) was demonstrated as the best dispersant for this kind of carbon nanostructure. With this procedure, long-term stability was assured to the dispersions, as demonstrated by long-term stability measurements performed for the water dispersions  and by size measurements performed in glycol dispersion 6 months after the preparation (Sani E et al, Potentialities of carbon nanohorn-based suspensions for solar thermal collectors, submitted ).
In view of their potential application in solar thermal collectors, a preliminary inspection of the dispersion stability at high temperature was performed. For this aim, we carried out 5 cycles of quick heating and cooling in a sealed vessel at various temperatures. As to the dispersions in water, for temperatures up to 120°C, a good stability was observed, while at higher temperatures some aggregation phenomena and a partial settling was detected. As to the glycol dispersions, considering the higher boiling point of the base fluid, a higher stability was observed up to 150°C, where only a weak aggregation started.
The result of these very preliminary high temperature stability studies shows that this is a critical facet. Investigations are in progress to improve the suspension stability at higher temperature for solar thermal applications, while in case of a standard solar water heater the observed stability seems already sufficient. It should be emphasized that these preliminary measurements have been performed for SWCNH suspensions without optimization of nanoparticle concentration or of nanoparticle/surfactant concentration ratio. It seems reasonable to expect that an optimized surfactant amount will considerably improve the nanofluid high temperature stability.
Scattering and absorption coefficients measurements
The experimental measurement of both absorption and scattering coefficients needs some additional definitions and the use of the diffusion equation. The details can be found in  and references therein. Here we will summarize only the basic facts.
where is the reduced scattering coefficient of the medium ( = μs (1 - g) with g anisotropy factor of the scattering function ) and μeff =(3 μa )1/2 is the effective attenuation coefficient.
we can obtain μeff as the slope of this linear relationship.
preparing a suspension with a previously calibrated diffusive medium having both high scattering and small absorption, in our case Intralipid-20% (Fresenius Kabi, Uppsala, Sweden);
then modifying the absorption properties of the overall suspension introducing very small quantities of SWCNH suspension that does not significantly modify the scattering property of the resulting fluid (nanofluid additions lower than 0.1%);
In this way, we were able to modify only the absorption properties of the suspension, without modifications of the scattering behaviour.
where μ generically labels the coefficient under investigation, ε is its respective value for the non-diluted suspension and ρ is the concentration of the absorbing/scattering medium within the resulting suspension.
where μa0 and are the known absorption and reduced scattering coefficient of the calibrated Intralipid suspension, and εanh the absorption coefficient of the original suspension of SWCNHs, before to dilute it in Intralipid suspension (as for the investigated concentration values of the original SWCNH suspension, the whole method was repeated for 5 samples with original concentrations ranging from 0.006 to 0.1 g/l).
The relationship between and ρnh is linear (Equation 7). Therefore, it is possible to obtain the absorption coefficient εanh as the slope divided by .
The experimental setup for fluence rate measurements in the infinite medium is composed by a chopped He-Ne laser (632.8 nm) which is introduced in the medium by means of an optical fibre whose extremity radiates isotropically in the medium. A second identical optical fibre mounted on a computer-controlled translator receives the radiation in correspondence of a set of fixed distances from the emitting fibre . The signal received by a photomultiplier coupled to the fibre is acquired by a lock-in amplifier.
The setup for transmittance measurement is composed by a calibrated length cell and by a chopped He-Ne laser. The light transmitted through the cell was measured with a photodiode and a lock-in amplifier. The experimental setup was similar to that of Ref.  with an acceptance angle of the detection system of 7 mrad. With this small acceptance angle the error on the extinction coefficient due to the unavoidable fraction of scattered received power was negligible, and the specific extinction coefficient has been obtained with an error smaller than 0.5%.
Therefore, the albedo of SWCNH suspension in water was only 0.05, confirming that the contribution of the scattered part to the total extinct light was very low. This value should be compared with those obtained in case of Indian ink aqueous suspensions, where the albedo was measured to be 0.15 . This favourably compares SWCHN suspensions with respect to more conventional black fluids employed in solar collectors also for their minimum scattering contribution to the total extinct light.
The small fraction of scattered light allows to easily estimate the light absorption by SWCNH-based nanofluids by means of simple spectrophotometric measurements.
Samples for spectrophotometric measurements
SWCNH Concentration (g/L)
From Figure 3 we can see that water and glycol show some spectral differences in their transmitting properties mainly for infrared wavelengths. SWCNHs produce a general decrease of the transmittance of the resulting nanofluid for almost all wavelengths and with a significant ultraviolet transmittance minimum due to nanoparticles. In general, glycol suspensions show a lower transmittance than water suspensions at fixed SWCNH concentration.
where α(λ) is the spectral absorption coefficient calculated from the transmittance spectra and I(λ) is the considered Sun spectrum.
Stored energy fraction F(r) for the various samples for different sunlight path lengths
SWCNH concentration (g/l)
Sample label (base fluid)
x= 1.0 cm (%)
x= 2.5 cm (%)
x= 5.0 cm (%)
x= 10.0 cm (%)
Pure base fluid
Pure base fluid
If the SWCNH concentration grows, the absorption within the fluid becomes more localized in the first layers. In fact, F(r) values are around 70% after 1 cm and more than 90% after 2.5 cm for 0.01 g/l concentration in both fluids, whereas for 0.02 g/l concentration, the absorption is around 90% after 1 cm and practically 100% for 2.5 cm. For the highest SWCNH concentration in Table 2 (0.05 g/l), the absorption is almost total within the first centimetre for both liquids.
This demonstrates the significant role of SWCNHs in considerably enhancing the sunlight absorption properties of the fluid.
As we can see, the absorption becomes more localized near the surface as the SWCNH concentration increases. Therefore, for a still fluid and in absence of any motion, a temperature gradient between the fluid lying near the surface and the fluid lying near the tube centre should be expected. Anyway, it should be emphasized that our simple model does not include any fluid motion or mixing. The aim of calculation in Equation 10 and Table 2 was to quantitatively evaluate the effect of SWCNHs on the absorption properties of the fluids, and not to show temperature distributions within the fluid. In fact, the still liquid is only an ideal approximation, as the real fluid will undergo both convective motions due to temperature gradients and a collective motion along the tube length due to external pumping. Both these effects, combined with the expected thermal conductivity enhancement due to SWCNHs similar to that observed in CNTs suspensions [16, 19], will contribute to uniform the fluid temperature for an optimal heat exchange.
This article reports on the characterization of SWCNH-based nanofluids for thermal solar applications. Preliminary thermal stability tests have been performed, showing that water-based suspensions are stable up to 120°C, while glycol-based suspensions are stable up to 150°C. An improvement of the thermal stability properties of the nanofluid should be expected by an optimization of SWCNH-surfactant concentration ratio.
As for the nanofluid optical properties, the described measurements show that nanohorn-based suspensions are very promising direct sunlight absorbers for thermal solar energy exploitation. We carried out both spectrally resolved and light scattering characterizations. We demonstrated that only small amount of radiation (~5% of the total extinction) was scattered by SWCNH particles and therefore the absorption effect was strongly prevailing. Moreover, the small scattering was also combined with an overall high absorption level at the sunlight emission wavelengths. Both these effects make SWCNHs-based nanofluids very appealing as direct absorbers in innovative solar collectors. The reported scattering and absorption properties can be used in simulations and nanofluid optimization.
single-wall carbon nanohorn
sodium n-dodecyl sulphate.
The work has been partially performed under the "Industria 2015" funding of the Italian Ministry of Economic Development.
- Eastman JA, Choi SUS, Li S, Yu W, Thompson LJ: Anomalously increased effective thermal conductivities of ethylene glycol-based nanofluids containing copper nanoparticles. Appl Phys Lett 2001, 78: 718–720. 10.1063/1.1341218View Article
- Xuan Y, Li Q: Heat transfer enhancement of nanofluids. Int J Heat Fluid Flow 2000, 21: 58–64. 10.1016/S0142-727X(99)00067-3View Article
- Heris SZ, Etemad SG, Esfahany MN: Experimental investigation of oxide nanofluids laminar flow convective heat transfer. Int Commun Heat Mass Transf 2006, 33: 529–535. 10.1016/j.icheatmasstransfer.2006.01.005View Article
- Xie H, Wang J, Xi TG, Liu Y, Ai F: Thermal conductivity enhancement of suspensions containing nanosized alumina particles. J Appl Phys 2002, 91: 4568–4572. 10.1063/1.1454184View Article
- Bergles AE: Recent development in convective heat transfer augmentation. Appl Mech Rev 1973, 26: 675–682.
- Ahuja AS: Augmentation of heat transport in laminar flow of polystyrene suspension: experiments and results. J Appl Phys 1975, 46: 3408–3416. 10.1063/1.322107View Article
- Fernandez-Garcìa A, Zarza E, Valenzuela L, Pérez M: Parabolic-trough solar collectors and their applications. Renew Sustain Energy Rev 2010, 14: 1695–1721.View Article
- Bertocchi R, Kribus A, Karni J: Experimentally determined optical properties of a polydisperse carbon black cloud for a solar particle receiver. J Sol Energy Eng 2004, 126: 833–841. 10.1115/1.1756924View Article
- Bertocchi R, Karni J, Kribus A: Experimental evaluation of a non-isothermal high temperature solar particle receiver. Energy 2004, 29: 687–700. 10.1016/j.energy.2003.07.001View Article
- Yuncu H, Paykoc E, Yener Y: Solar energy utilization. Dordrecht: Kluwer Academic Publishers; 1987.View Article
- Tyagi H, Phelan P, Prasher R: Predicted efficiency of a nanofluid-based direct absorption solar receiver. In Proceedings of ES2007, Energy Sustainability 2007: June 27–30. California: Long Beach; 2007.
- Kim P, Shi L, Majumdar A, McEuen PL: Thermal transport measurements of individual multiwalled nanotubes. Phys Rev Lett 2001, 87: 215502–1-215502–4.
- Natarajan E, Sathish R: Role of nanofluids in solar water heater. Int J Adv Manuf Technol 2009.
- Choi SUS, Zhang ZG, Yu W, Lockwood FE, Grulke EA: Anomalous thermal conductivity enhancement in nanotube suspensions. Appl Phys Lett 2001, 79: 2252–2254. 10.1063/1.1408272View Article
- Assael MJ, Chen CF, Metaxa I, Wakeham WA: Thermal conductivity of suspensions of carbon nanotubes in water. Int J Thermophys 2004, 25: 971–985. 10.1023/B:IJOT.0000038494.22494.04View Article
- Marquis FDS, Chibante LPF: Improving the heat transfer of nanofluids and nanolubrificants with carbon nanotubes. J Miner Met Mater Soc 2005, 57: 32–43.View Article
- Hone J, Whitney M, Zettl A: Thermal conductivity of single-walled carbon nanotubes. Synth Met 1999, 103: 2498–2499. 10.1016/S0379-6779(98)01070-4View Article
- Berber S, Kwon YK, Tomànek D: Unusually high thermal conductivity of carbon nanotubes. Phys Rev Lett 2000, 84: 4613–4616. 10.1103/PhysRevLett.84.4613View Article
- Ding Y, Alias H, Wen D, Williams RA: Heat transfer of aqueous suspensions of carbon nanotubes (CNT nanofluids). Int J Heat Mass Transf 2006, 49: 240–250. 10.1016/j.ijheatmasstransfer.2005.07.009View Article
- Iijima S, Yudasaka M, Yamada R, Bandow S, Suenaga K, Kokai F, Takahashi K: Nano-aggregates of single-walled graphitic carbon nano-horns. Chem Phys Lett 1999, 309: 165–170. 10.1016/S0009-2614(99)00642-9View Article
- Fan X, Tan J, Zhang G, Zhang F: Isolation of carbon nanohorn assemblies and their potential for intracellular delivery. Nanotechnology 2007, 18: 195103–1-195103–6. 10.1088/0957-4484/18/19/195103View Article
- Yoshitake YT, Shimakawa Y, Kuroshima S, Kimura H, Ichihashi T, Kubo Y, Kasuya D, Takahashi K, Kokai F, Yudasaka M, Iijima S: Preparation of fine platinum catalyst supported on single-wall carbon nanohorns for fuel cell application. Physica B 2002, 323: 124–126. 10.1016/S0921-4526(02)00871-2View Article
- Bekyarova E, Murata K, Yudasaka M, Kasuya D, Iijima S, Tanaka H, Kanoh H, Kaneko K: Single-wall nanostructured carbon for methane storage. J Phys Chem B 2003, 107: 4682–4684.
- Murakami T, Ajima K, Miyawaki J, Yudasaka M, Iijima S, Shiba K: Drug-loaded carbon nanohorns: adsorption and release of dexamethasone in vitro. Mol Pharm 2004, 1: 399–405. 10.1021/mp049928eView Article
- Ajima K, Yudasaka M, Murakami T, Maigne A, Shiba K, Iijima S: Carbon nanohorns as anticancer drug carriers. Mol Pharm 2005, 2: 475–480. 10.1021/mp0500566View Article
- Murakami T, Fan J, Yudasaka M, Iijima S, Shiba K: Solubilization of single-wall carbon nanohorns using a PEG-doxorubicin conjugate. Mol Pharm 2006, 3: 408–414. 10.1021/mp060027aView Article
- Krungleviciute V, Migone AD, Pepka M: Characterization of single-walled carbon nanohorns using neon adsorption isotherms. Carbon 2009, 47: 769–774. 10.1016/j.carbon.2008.11.036View Article
- Murata K, Kaneko K, Kokai F, Takahashi K, Yudasaka M, Iijima S: Pore structure of single-wall carbon nanohorn aggregates. Chem Phys Lett 2000, 331: 14–20. 10.1016/S0009-2614(00)01152-0View Article
- Yudasaka M, Iijima S, Crespi VH: Single-wall carbon nanohorns and nanocones. Top Appl Phys 2008, 111: 605–629. full_textView Article
- Kasuya D, Yudasaka M, Takahashi K, Kokai F, Ilijima S: Selective production of single-wall carbon nanohorn aggregates and their formation mechanism. J Phys Chem B 2002, 106: 4947–4951. 10.1021/jp020387nView Article
- Delgado JL, Herranz MA, Martin N: The nano-forms of carbon. J Mater Chem 2008, 18: 1417–1426. 10.1039/b717218dView Article
- Azami T, Yuge R, Kasuya D, Yoshitake T, Kubo Y, Yudasaka M, Iijima A: Large scale production of SWNH. The 32nd Fullerene-Nanotubes General Symposium 2007, 3–20.
- Pagona G, Sandanayaka ASD, Araki Y, Fan J, Tagmatarchis N, Yudasaka M, Iijima S, Ito O: Electronic interplay on illuminated aqueous carbon nanohorn-porphyrin ensembles. J Phys Chem B 2006, 110: 20729–20732. 10.1021/jp064685mView Article
- Lynch RM, Voy BH, Glass DF, Mahurin SM, Zhao B, Hu H, Saxton AM, Donnell RL, Cheng MD: Assessing the pulmonary toxicity of single-walled carbon nanohorns. Nanotoxicology 2007, 2: 157–166. 10.1080/17435390701598496View Article
- Das SK, Putra N, Roetzel W: Pool boiling characteristics of nano-fluids. Int J Heat Mass Transf 2003, 46: 851–862. 10.1016/S0017-9310(02)00348-4View Article
- Park K, Jung D, Shim SE: Nucleate boiling heat transfer in aqueous solutions with carbon nanotubes up to critical heat fluxes. Int J Multiphase Flow 2009, 35: 525–532. 10.1016/j.ijmultiphaseflow.2009.02.015View Article
- Park K, Jung D: Boiling heat transfer enhancement with carbon nanotubes for refrigerants used in building air-conditioning. Energy Build 2007, 39: 1061–1064. 10.1016/j.enbuild.2006.12.001View Article
- Sani E, Barison S, Pagura C, Mercatelli L, Sansoni P, Fontani D, Jafrancesco D, Francini F: Carbon nanohorns-based nanofluids as direct sunlight absorbers. OpEx 2010, 18: 5179–5187. 10.1364/OE.18.005179
- Schiavon M: Device and method for production of carbon nanotubes, fullerene and their derivatives. U.S. Patent 7,125,525; EP 1428794 U.S. Patent 7,125,525; EP 1428794
- Pagura C, Barison S, Battiston S, Schiavon M: Synthesis and characterization of single wall carbon nanohorns produced by direct vaporization of graphite. In Proceeding of TechConnect World. Volume 1. Anaheim, CA: Advanced Materials, CNTs, Particles, Films and Composites; 2010:289–291.
- Fedele L, Colla L, Bobbo S, Barison S, Agresti F: Experimental stability analysis of different water-based nanofluids. Nanoscale Research Letters; 2011:in press.
- Martelli F, Bassani M, Alianelli L, Zangheri L, Zaccanti G: Accuracy of the diffusion equation to describe photon migration through an infinite medium: numerical and experimental investigation. Phys Med Biol 2000, 45: 1359–1373. 10.1088/0031-9155/45/5/318View Article
- Zaccanti G, Del Bianco S, Martelli F: Measurements of optical properties of high density media. Appl Opt 2003, 42: 4023–4030. 10.1364/AO.42.004023View Article
- Martelli F, Zaccanti G: Calibration of scattering and absorption properties of a liquid diffusive medium at NIR wavelengths. CW method. Opt Exp 2007, 15: 486–500. 10.1364/OE.15.000486View Article
- Wagner TR, Houf WG, Incropera FP: Radiative property measurements for India ink suspensions of varying concentration. Sol Energy 1980, 25: 549–554. 10.1016/0038-092X(80)90089-4View Article
- CIE Technical Report no. 85: Solar Spectral Irradiance. 1989.
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.